Download presentation

Presentation is loading. Please wait.

Published byVivien Booth Modified about 1 year ago

1
Diffusion in multicomponent solids Anton Van der Ven Department of Materials Science and Engineering University of Michigan Ann Arbor, MI

2
Coarse graining time Diffusion in a crystal Two levels of time coarse graining

3
Coarse graining time Diffusion in a crystal Two levels of time coarse graining Short-time coarse graining: transition state theory - MD simulations - Harmonic approximation Vineyard, J. Phys. Chem. Solids 3, 121 (1957).

4
Coarse graining time Diffusion in a crystal Two levels of time coarse graining Short-time coarse graining: transition state theory - MD simulations - Harmonic approximation A second level of coarse graining that leads to Fick’s law Green-Kubo Kinetic coefficients derived from fluctuations at equilibrium Vineyard, J. Phys. Chem. Solids 3, 121 (1957). Zwanzig, Annu. Rev. Phys. Chem. 16, 67 (1965).

5
Interstitial diffusion C diffusion in bcc Iron (steel) Li diffusion in transition metal oxide host O diffusion on Pt-(111) surface In all examples, diffusion occurs on a rigid lattice which is externally imposed by a host or substrate

6
Example of interstitial diffusion

7
Irreversible thermodynamics: interstitial diffusion of one component

8
Notation M = number of lattice sites N = number of diffusing atoms v s = volume per lattice site x = N/M C=x/v s

9
Interstitial diffusion: one component Kubo-Green relations (linear response statistical mechanics) Thermodynamic factor Kinetic coefficient A. Van der Ven, G. Ceder, Handbook of Materials Modeling, chapt. 1.17, Ed. S. Yip, Springer (2005). R. Gomer, Rep. Prog. Phys. 53, 917 (1990)/

10
Trajectories

11
More familiar form Thermodynamic factor Self diffusion coefficient R. Gomer, Rep. Prog. Phys. 53, 917 (1990)/

12
Common approximation Thermodynamic factor Tracer diffusion coefficient R. Gomer, Rep. Prog. Phys. 53, 917 (1990)/

13
Diffusion coefficient at 300 K Thermodynamic factor A. Van der Ven, G. Ceder, M. Asta, P.D. Tepesch, Phys Rev. B 64 (2001)

14
Interstitial diffusion (two components) C & N diffusion in bcc Iron (steel) Li & Na diffusion in transition metal oxide host O & S diffusion on Pt-(111) surface In all examples, diffusion occurs on a rigid lattice which is externally imposed by a host or substrate

15
Diffusion of two species on a lattice

16
Alternative factorization Kubo-Green A. Van der Ven, G. Ceder, Handbook of Materials Modeling, chapt. 1.17, Ed. S. Yip, Springer (2005). A.R. Allnatt, A.B. Lidiard, Atomic Transport in Solids (Cambridge Univ. Press, 1993).

17
Kinetic coefficients (fcc lattice in dilute vacancy limit, ideal solution)

18
Diffusion in an alloy: substitutional diffusion Not interstitial diffusion Instead, diffusing atoms form the lattice Dilute concentration of vacancies

19
Thermodynamic driving forces for substitutional diffusion A. Van der Ven, G. Ceder, Handbook of Materials Modeling, chapt. 1.17, Ed. S. Yip, Springer (2005).

20
Textbook treatment of substitional diffusion Not Rigorous

21
Traditional Gibbs-Duhem Assume vacancy concentration in equilibrium everywhere

22
Textbook treatment of substitional diffusion Not Rigorous Traditional Gibbs-Duhem Rigorous Assume vacancy concentration in equilibrium everywhere

23
Lattice frame and laboratory frame of reference Fluxes in the laboratory frame

24
Lattice frame and laboratory frame of reference Fluxes in the laboratory frame Drift Interdiffusion

25
Rigorous treatment

26
Diagonalize the D-matrix Yields a mode corresponding to (a) density relaxation (b) interdiffusion K. W. Kehr, et al, Phys. Rev. B 39, 4891 (1989) Rigorous treatment

27
Physical meaning of modes + and -

28
Density fluctuations relax with a time constant of + K. W. Kehr, et al, Phys. Rev. B 39, 4891 (1989)

29
Physical meaning of modes + and - Density fluctuations relax with a time constant of + Compositional inhomogeneities decay with a time constant of K. W. Kehr, et al, Phys. Rev. B 39, 4891 (1989)

30
Comparisons of different treatments B =10x A Random alloy B =100x A Traditional and rigorous treatment are equivalent only when B = A

31
Example: Li x CoO 2

32
Intercalation Oxide as Cathode in Rechargeable Lithium Battery Li x CoO 2

33
Cluster Expansions First-Principles (Density Functional Theory) Fit V , V , V , … to first-principles energies Monte Carlo

34

35
First principles energies (LDA) of different lithium-vacancy configurations A. Van der Ven, et al, Phys. Rev. B 58 (6), p (1998).

36
Cluster expansion for Li x CoO 2 A. Van der Ven, et al, Phys. Rev. B 58 (6), p (1998).

37
Calculated Li x CoO 2 phase diagram A. Van der Ven, et al, Phys. Rev. B 58 (6), p (1998).

38
Calculated phase diagram Experimental phase diagram Reimers, Dahn, J.Electrochem. Soc, (1992) Ohzuku, Ueda, J. Electrochem. Soc. (1994) Amatucci et al, J. Electrochem. Soc. (1996)

39
Predicted phases confirmed experimentally Confirmed experimentally with TEM Y. Shao-Horn, S. Levasseur, F. Weill, C. Delmas, J. Electrochem. Soc. 150 (2003), A 366

40
Predicted phases confirmed experimentally Confirmed experimentally with TEM Y. Shao-Horn, S. Levasseur, F. Weill, C. Delmas, J. Electrochem. Soc. 150 (2003), A 366 Confirmed experimentally by Z. Chen, Z. Lu, J.R. Dahn J. Electrochem. Soc. 149, A1604 (2002)

41
Calculated phase diagram Experimental phase diagram ? Reimers, Dahn, J.Electrochem. Soc, (1992) Ohzuku, Ueda, J. Electrochem. Soc. (1994) Amatucci et al, J. Electrochem. Soc. (1996) M. Menetrier et al J. Mater Chem. 9, 1135 (1999)

42
Effect of metal insulator transition Holes in the valence band localize in space LDA & GGA fails to accurately describe localized electronic states C. A. Marianetti et al, Nature Materials, 3, 627 (2004).

43
Diffusion Fick’s Law

44
Interstitial diffusion and configurational disorder Kubo-Green relations Thermodynamic factor Self diffusion coefficient

45
Individual hops: Transition state theory

46
Kinetically resolved activation barrier A. Van der Ven, G. Ceder, M. Asta, P.D. Tepesch, Phys Rev. B 64 (2001)

47
Migration mechanism in Li x CoO 2 Single vacancy hop mechanism Divacancy hop Mechanism Oxygen Cobalt Lithium

48
Single vacancy hop Divacancy hop Oxygen Cobalt Lithium

49
Many types of hop possibilities in the lithium plane

50
Migration barriers depend configuration and concentration Divacancy mechanism Single-vacancy mechanism

51
Local Cluster expansion for divacancy migration barrier

52
Calculated diffusion coefficient (First Principles cluster expansion + kinetic Monte Carlo) Diffusion coefficient at 300 K Thermodynamic factor A. Van der Ven, G. Ceder, M. Asta, P.D. Tepesch, Phys Rev. B 64 (2001)

53
Available migration mechanisms for each lithium ion Channels into a divacancy Number of vacancies around lithium Channels into isolated vacancies

54
Diffusion occurs with a divacancy mechanism

55
Diffusion and phase transformations in Al-Li alloys Dark field TEM A. Kalogeridis, J. Pesieka, E. Nembach, Acta Mater 47 (1999) 1953 Dark field in situ TEM, peak aged Al-Li specimen under full load H. Rosner, W. Liu, E. Nembach, Phil Mag A, 79 (1999) 2935

56
fcc Al-Li alloy Binary cluster expansion Li at site i Al at site i Fit to LDA energies of 70 different Al-Li arrangements on fcc A. Van der Ven, G. Ceder, Phys. Rev. B71, (2005)

57
Calculated thermodynamic and kinetic properties of Al-Li alloy First principles cluster expansion + Monte Carlo A. Van der Ven, G. Ceder, Phys. Rev. B71, (2005)

58
Expand environment dependence of vacancy formation energy Fit to 23 vacancy LDA formation energies in different Al-Li arrangements (107 atom supercells). Li at site i Al at site i Local cluster expansion* (perturbation to binary cluster expansion) A. Van der Ven, G. Ceder, Phys. Rev. B71, (2005)

59
Equilibrium vacancy concentration (Monte Carlo applied to cluster expansion) A. Van der Ven, G. Ceder, Phys. Rev. B71, (2005)

60
Vacancy surrounds itself by Al Short range order around a vacancy 750 Kelvin A. Van der Ven, G. Ceder, Phys. Rev. B71, (2005)

61
Vacancies reside on lithium sublattice in L12 Al Li 600 Kelvin

62
Migration barriers for lithium and aluminum differ by ~150 meV Li barriers Al barriers Calculated (LDA) in 107 atom supercells

63
Al Li Calculated interdiffusion coefficient A. Van der Ven, G. Ceder, Phys. Rev. Lett. 94, (2005).

64
Hop mechanisms

65
Frequency of hop angles between successive hops A. Van der Ven, G. Ceder, Phys. Rev. Lett. 94, (2005).

66
Conclusion Green-Kubo formalism yields rigorous expressions for diffusion coefficients Discussed diffusion formalism for both interstitial and substitutional diffusion Intriguing hop mechanisms in multi- component solids that can depend on ordering Thermodynamics plays a crucial role!

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google